#------------------------------------------------------------------------------
#$Date: 2015-06-04 14:08:30 +0300 (Thu, 04 Jun 2015) $
#$Revision: 137932 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/31/4343183.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4343183
loop_
_publ_author_name
'Yang, Lin'
'Pisoni, Andrea'
'Magrez, Arnaud'
'Katrych, Sergiy'
'Arakcheeva, Alla'
'Dalla Piazza, Bastien'
'Prša, Krunoslav'
'Jaćimović, Jaćim'
'Akrap, Ana'
'Teyssier, Jérémie'
'Forró, László'
'Rønnow, Henrik M'
_publ_section_title
;
 Crystal Structure, Transport, and Magnetic Properties of an Ir(6+)
 Compound Ba8Al2IrO14.
;
_journal_issue                   9
_journal_name_full               'Inorganic chemistry'
_journal_page_first              4371
_journal_page_last               4376
_journal_paper_doi               10.1021/acs.inorgchem.5b00157
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         '2(Al O4), Ir O6, 8(Ba)'
_chemical_formula_sum            'Al2 Ba8 Ir O14'
_chemical_formula_weight         1568.88
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 109.656(5)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   19.8283(15)
_cell_length_b                   5.9591(5)
_cell_length_c                   7.6013(5)
_cell_measurement_temperature    90(2)
_cell_volume                     845.82(11)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      90(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0537
_diffrn_reflns_av_sigmaI/netI    0.0370
_diffrn_reflns_limit_h_max       30
_diffrn_reflns_limit_h_min       -32
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            12095
_diffrn_reflns_theta_full        35.00
_diffrn_reflns_theta_max         35.00
_diffrn_reflns_theta_min         3.59
_exptl_absorpt_coefficient_mu    26.297
_exptl_absorpt_correction_T_max  0.4370
_exptl_absorpt_correction_T_min  0.1699
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.160
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'needle like'
_exptl_crystal_F_000             1326
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         4.652
_refine_diff_density_min         -7.287
_refine_diff_density_rms         0.471
_refine_ls_extinction_coef       0.00027(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.110
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     64
_refine_ls_number_reflns         2014
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.110
_refine_ls_R_factor_all          0.0455
_refine_ls_R_factor_gt           0.0392
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0156P)²+51.8678P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0791
_refine_ls_wR_factor_ref         0.0821
_reflns_number_gt                1820
_reflns_number_total             2014
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic5b00157_si_001.cif
_cod_data_source_block           lt
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Empirical' changed to
'empirical' according to
/usr/data/users/saulius/crontab/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 
;
_cod_database_code               4343183
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ir1 Ir 0.0000 0.0000 0.0000 0.00704(10) Uani 1 4 d S
Ba1 Ba 0.47474(3) 0.0000 0.20736(8) 0.01131(12) Uani 1 2 d S
Ba2 Ba 0.31481(3) 0.0000 0.70665(8) 0.01179(12) Uani 1 2 d S
Ba3 Ba 0.17257(3) 0.0000 0.98942(10) 0.01794(14) Uani 1 2 d S
Ba4 Ba 0.09747(4) 0.0000 0.46073(10) 0.02508(17) Uani 1 2 d S
Al1 Al 0.3265(3) 0.0000 0.2965(6) 0.0286(9) Uani 1 2 d S
O1 O 0.4076(7) 0.0000 0.4694(14) 0.041(3) Uani 1 2 d S
O2 O 0.0336(4) 0.0000 0.7750(10) 0.0116(12) Uani 1 2 d S
O3 O 0.0726(3) 0.2277(9) 0.1226(7) 0.0126(9) Uani 1 1 d .
O4 O 0.3271(6) 0.0000 0.0724(16) 0.054(4) Uani 1 2 d S
O5a O 0.1980(11) 0.1898(15) 0.7185(14) 0.055(4) Uiso 0.50 1 d P
O5b O 0.2859(10) 0.2186(8) 0.3443(15) 0.055(4) Uiso 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ir Ir -1.4442 7.9887 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ir1 O3 180.0(5) 5 .
O3 Ir1 O3 87.1(3) 5 2
O3 Ir1 O3 92.9(3) . 2
O3 Ir1 O3 92.9(3) 5 6
O3 Ir1 O3 87.1(3) . 6
O3 Ir1 O3 180.0(2) 2 6
O3 Ir1 O2 90.2(2) 5 5_556
O3 Ir1 O2 89.8(2) . 5_556
O3 Ir1 O2 90.2(2) 2 5_556
O3 Ir1 O2 89.8(2) 6 5_556
O3 Ir1 O2 89.8(2) 5 1_554
O3 Ir1 O2 90.2(2) . 1_554
O3 Ir1 O2 89.8(2) 2 1_554
O3 Ir1 O2 90.2(2) 6 1_554
O2 Ir1 O2 180.0(3) 5_556 1_554
O3 Ir1 Ba4 55.82(15) 5 5
O3 Ir1 Ba4 124.18(15) . 5
O3 Ir1 Ba4 55.82(15) 2 5
O3 Ir1 Ba4 124.18(15) 6 5
O2 Ir1 Ba4 129.5(2) 5_556 5
O2 Ir1 Ba4 50.5(2) 1_554 5
O3 Ir1 Ba4 124.18(15) 5 .
O3 Ir1 Ba4 55.82(15) . .
O3 Ir1 Ba4 124.18(15) 2 .
O3 Ir1 Ba4 55.82(15) 6 .
O2 Ir1 Ba4 50.5(2) 5_556 .
O2 Ir1 Ba4 129.5(2) 1_554 .
Ba4 Ir1 Ba4 180.000(14) 5 .
O3 Ir1 Ba3 55.83(15) 5 5_556
O3 Ir1 Ba3 124.17(15) . 5_556
O3 Ir1 Ba3 55.83(15) 2 5_556
O3 Ir1 Ba3 124.17(15) 6 5_556
O2 Ir1 Ba3 51.1(2) 5_556 5_556
O2 Ir1 Ba3 128.9(2) 1_554 5_556
Ba4 Ir1 Ba3 78.37(2) 5 5_556
Ba4 Ir1 Ba3 101.63(2) . 5_556
O3 Ir1 Ba3 124.17(15) 5 1_554
O3 Ir1 Ba3 55.83(15) . 1_554
O3 Ir1 Ba3 124.17(15) 2 1_554
O3 Ir1 Ba3 55.83(15) 6 1_554
O2 Ir1 Ba3 128.9(2) 5_556 1_554
O2 Ir1 Ba3 51.1(2) 1_554 1_554
Ba4 Ir1 Ba3 101.63(2) 5 1_554
Ba4 Ir1 Ba3 78.37(2) . 1_554
Ba3 Ir1 Ba3 180.0 5_556 1_554
O3 Ir1 Ba1 127.58(15) 5 3_455
O3 Ir1 Ba1 52.42(15) . 3_455
O3 Ir1 Ba1 55.36(15) 2 3_455
O3 Ir1 Ba1 124.64(15) 6 3_455
O2 Ir1 Ba1 58.804(11) 5_556 3_455
O2 Ir1 Ba1 121.196(11) 1_554 3_455
Ba4 Ir1 Ba1 110.439(11) 5 3_455
Ba4 Ir1 Ba1 69.561(11) . 3_455
Ba3 Ir1 Ba1 72.233(11) 5_556 3_455
Ba3 Ir1 Ba1 107.767(11) 1_554 3_455
O3 Ir1 Ba1 52.42(15) 5 7_545
O3 Ir1 Ba1 127.58(15) . 7_545
O3 Ir1 Ba1 124.64(15) 2 7_545
O3 Ir1 Ba1 55.36(15) 6 7_545
O2 Ir1 Ba1 121.196(11) 5_556 7_545
O2 Ir1 Ba1 58.804(11) 1_554 7_545
Ba4 Ir1 Ba1 69.561(11) 5 7_545
Ba4 Ir1 Ba1 110.439(11) . 7_545
Ba3 Ir1 Ba1 107.767(11) 5_556 7_545
Ba3 Ir1 Ba1 72.233(11) 1_554 7_545
Ba1 Ir1 Ba1 180.00(2) 3_455 7_545
O1 Ba1 O4 63.7(4) . .
O1 Ba1 O1 79.9(4) . 5_656
O4 Ba1 O1 143.6(4) . 5_656
O1 Ba1 O3 135.96(17) . 8
O4 Ba1 O3 130.79(19) . 8
O1 Ba1 O3 76.0(2) 5_656 8
O1 Ba1 O3 135.96(17) . 3_545
O4 Ba1 O3 130.79(19) . 3_545
O1 Ba1 O3 76.0(2) 5_656 3_545
O3 Ba1 O3 71.8(2) 8 3_545
O1 Ba1 O3 122.6(2) . 4_545
O4 Ba1 O3 71.4(2) . 4_545
O1 Ba1 O3 135.11(19) 5_656 4_545
O3 Ba1 O3 100.19(13) 8 4_545
O3 Ba1 O3 60.86(18) 3_545 4_545
O1 Ba1 O3 122.6(2) . 7
O4 Ba1 O3 71.4(2) . 7
O1 Ba1 O3 135.11(19) 5_656 7
O3 Ba1 O3 60.86(18) 8 7
O3 Ba1 O3 100.19(13) 3_545 7
O3 Ba1 O3 68.9(2) 4_545 7
O1 Ba1 O2 85.39(14) . 7_546
O4 Ba1 O2 87.05(14) . 7_546
O1 Ba1 O2 90.18(14) 5_656 7_546
O3 Ba1 O2 130.46(17) 8 7_546
O3 Ba1 O2 58.66(17) 3_545 7_546
O3 Ba1 O2 57.89(17) 4_545 7_546
O3 Ba1 O2 126.61(17) 7 7_546
O1 Ba1 O2 85.39(14) . 7_556
O4 Ba1 O2 87.05(14) . 7_556
O1 Ba1 O2 90.18(14) 5_656 7_556
O3 Ba1 O2 58.66(17) 8 7_556
O3 Ba1 O2 130.46(17) 3_545 7_556
O3 Ba1 O2 126.61(17) 4_545 7_556
O3 Ba1 O2 57.89(17) 7 7_556
O2 Ba1 O2 170.6(3) 7_546 7_556
O1 Ba1 Al1 31.8(3) . .
O4 Ba1 Al1 31.9(3) . .
O1 Ba1 Al1 111.7(3) 5_656 .
O3 Ba1 Al1 143.87(10) 8 .
O3 Ba1 Al1 143.87(10) 3_545 .
O3 Ba1 Al1 97.49(12) 4_545 .
O3 Ba1 Al1 97.49(12) 7 .
O2 Ba1 Al1 85.55(13) 7_546 .
O2 Ba1 Al1 85.55(13) 7_556 .
O1 Ba1 Ir1 120.47(3) . 3_545
O4 Ba1 Ir1 97.34(13) . 3_545
O1 Ba1 Ir1 101.28(13) 5_656 3_545
O3 Ba1 Ir1 100.22(11) 8 3_545
O3 Ba1 Ir1 34.35(10) 3_545 3_545
O3 Ba1 Ir1 34.41(10) 4_545 3_545
O3 Ba1 Ir1 98.20(10) 7 3_545
O2 Ba1 Ir1 35.59(14) 7_546 3_545
O2 Ba1 Ir1 153.00(14) 7_556 3_545
Al1 Ba1 Ir1 111.97(3) . 3_545
O1 Ba1 Ir1 120.47(3) . 3
O4 Ba1 Ir1 97.34(13) . 3
O1 Ba1 Ir1 101.28(13) 5_656 3
O3 Ba1 Ir1 34.35(10) 8 3
O3 Ba1 Ir1 100.22(11) 3_545 3
O3 Ba1 Ir1 98.20(10) 4_545 3
O3 Ba1 Ir1 34.41(10) 7 3
O2 Ba1 Ir1 153.00(14) 7_546 3
O2 Ba1 Ir1 35.59(14) 7_556 3
Al1 Ba1 Ir1 111.97(3) . 3
Ir1 Ba1 Ir1 117.521(17) 3_545 3
O5b Ba2 O5b 82.795(18) 4_546 7_556
O5b Ba2 O5a 19.071(4) 4_546 6
O5b Ba2 O5a 68.209(15) 7_556 6
O5b Ba2 O5a 68.209(15) 4_546 .
O5b Ba2 O5a 19.071(4) 7_556 .
O5a Ba2 O5a 51.434(12) 6 .
O5b Ba2 O4 87.20(18) 4_546 1_556
O5b Ba2 O4 87.20(18) 7_556 1_556
O5a Ba2 O4 74.8(2) 6 1_556
O5a Ba2 O4 74.8(2) . 1_556
O5b Ba2 O3 161.48(11) 4_546 7_556
O5b Ba2 O3 99.03(11) 7_556 7_556
O5a Ba2 O3 147.28(11) 6 7_556
O5a Ba2 O3 108.79(11) . 7_556
O4 Ba2 O3 74.5(2) 1_556 7_556
O5b Ba2 O3 99.03(11) 4_546 4_546
O5b Ba2 O3 161.48(11) 7_556 4_546
O5a Ba2 O3 108.79(11) 6 4_546
O5a Ba2 O3 147.28(11) . 4_546
O4 Ba2 O3 74.5(2) 1_556 4_546
O3 Ba2 O3 73.5(2) 7_556 4_546
O5b Ba2 O5b 70.531(12) 4_546 6
O5b Ba2 O5b 104.83(2) 7_556 6
O5a Ba2 O5b 86.810(14) 6 6
O5a Ba2 O5b 109.33(2) . 6
O4 Ba2 O5b 152.69(6) 1_556 6
O3 Ba2 O5b 125.90(11) 7_556 6
O3 Ba2 O5b 93.05(11) 4_546 6
O5b Ba2 O5b 104.83(2) 4_546 .
O5b Ba2 O5b 70.531(12) 7_556 .
O5a Ba2 O5b 109.33(2) 6 .
O5a Ba2 O5b 86.810(14) . .
O4 Ba2 O5b 152.69(6) 1_556 .
O3 Ba2 O5b 93.05(11) 7_556 .
O3 Ba2 O5b 125.90(11) 4_546 .
O5b Ba2 O5b 52.918(12) 6 .
O5b Ba2 O1 121.51(14) 4_546 .
O5b Ba2 O1 121.51(14) 7_556 .
O5a Ba2 O1 139.30(16) 6 .
O5a Ba2 O1 139.30(16) . .
O4 Ba2 O1 139.6(3) 1_556 .
O3 Ba2 O1 73.3(2) 7_556 .
O3 Ba2 O1 73.3(2) 4_546 .
O5b Ba2 O1 52.76(18) 6 .
O5b Ba2 O1 52.76(18) . .
O5b Ba2 Al1 99.34(7) 4_546 .
O5b Ba2 Al1 99.34(7) 7_556 .
O5a Ba2 Al1 112.93(8) 6 .
O5a Ba2 Al1 112.93(8) . .
O4 Ba2 Al1 171.2(3) 1_556 .
O3 Ba2 Al1 98.54(13) 7_556 .
O3 Ba2 Al1 98.54(13) 4_546 .
O5b Ba2 Al1 30.52(4) 6 .
O5b Ba2 Al1 30.52(4) . .
O1 Ba2 Al1 31.7(2) . .
O5b Ba2 Ba3 120.57(2) 4_546 7_557
O5b Ba2 Ba3 56.717(12) 7_556 7_557
O5a Ba2 Ba3 101.573(18) 6 7_557
O5a Ba2 Ba3 60.447(12) . 7_557
O4 Ba2 Ba3 53.091(12) 1_556 7_557
O3 Ba2 Ba3 49.62(11) 7_556 7_557
O3 Ba2 Ba3 107.99(11) 4_546 7_557
O5b Ba2 Ba3 153.020(16) 6 7_557
O5b Ba2 Ba3 100.295(11) . 7_557
O1 Ba2 Ba3 116.68(10) . 7_557
Al1 Ba2 Ba3 126.275(16) . 7_557
O5a Ba3 O2 87.19(14) 6 .
O5a Ba3 O2 87.19(14) . .
O5a Ba3 O3 115.23(11) 6 6_556
O5a Ba3 O3 148.09(10) . 6_556
O2 Ba3 O3 61.48(16) . 6_556
O5a Ba3 O3 148.09(10) 6 1_556
O5a Ba3 O3 115.23(11) . 1_556
O2 Ba3 O3 61.48(16) . 1_556
O3 Ba3 O3 56.8(2) 6_556 1_556
O5a Ba3 O4 72.2(2) 6 1_556
O5a Ba3 O4 72.2(2) . 1_556
O2 Ba3 O4 156.9(3) . 1_556
O3 Ba3 O4 136.8(2) 6_556 1_556
O3 Ba3 O4 136.8(2) 1_556 1_556
O5a Ba3 O4 54.8(2) 6 7_546
O5a Ba3 O4 107.6(2) . 7_546
O2 Ba3 O4 87.8(2) . 7_546
O3 Ba3 O4 67.9(3) 6_556 7_546
O3 Ba3 O4 124.3(3) 1_556 7_546
O4 Ba3 O4 88.6(2) 1_556 7_546
O5a Ba3 O4 107.6(2) 6 7_556
O5a Ba3 O4 54.8(2) . 7_556
O2 Ba3 O4 87.8(2) . 7_556
O3 Ba3 O4 124.3(3) 6_556 7_556
O3 Ba3 O4 67.9(3) 1_556 7_556
O4 Ba3 O4 88.6(2) 1_556 7_556
O4 Ba3 O4 162.0(5) 7_546 7_556
O5a Ba3 O5b 126.71(2) 6 1_556
O5a Ba3 O5b 103.328(15) . 1_556
O2 Ba3 O5b 143.97(11) . 1_556
O3 Ba3 O5b 105.85(11) 6_556 1_556
O3 Ba3 O5b 83.13(10) 1_556 1_556
O4 Ba3 O5b 54.5(2) 1_556 1_556
O4 Ba3 O5b 120.2(2) 7_546 1_556
O4 Ba3 O5b 71.8(2) 7_556 1_556
O5a Ba3 O5b 103.328(15) 6 6_556
O5a Ba3 O5b 126.71(2) . 6_556
O2 Ba3 O5b 143.97(11) . 6_556
O3 Ba3 O5b 83.13(10) 6_556 6_556
O3 Ba3 O5b 105.85(10) 1_556 6_556
O4 Ba3 O5b 54.5(2) 1_556 6_556
O4 Ba3 O5b 71.8(2) 7_546 6_556
O4 Ba3 O5b 120.2(2) 7_556 6_556
O5b Ba3 O5b 48.796(12) 1_556 6_556
O5a Ba3 Al1 101.13(7) 6 1_556
O5a Ba3 Al1 101.13(7) . 1_556
O2 Ba3 Al1 170.69(17) . 1_556
O3 Ba3 Al1 110.59(12) 6_556 1_556
O3 Ba3 Al1 110.59(12) 1_556 1_556
O4 Ba3 Al1 32.4(2) 1_556 1_556
O4 Ba3 Al1 93.6(2) 7_546 1_556
O4 Ba3 Al1 93.6(2) 7_556 1_556
O5b Ba3 Al1 30.02(4) 1_556 1_556
O5b Ba3 Al1 30.02(4) 6_556 1_556
O5a Ba3 Ir1 119.16(2) 6 1_556
O5a Ba3 Ir1 119.16(2) . 1_556
O2 Ba3 Ir1 36.08(15) . 1_556
O3 Ba3 Ir1 34.81(10) 6_556 1_556
O3 Ba3 Ir1 34.81(10) 1_556 1_556
O4 Ba3 Ir1 167.0(2) 1_556 1_556
O4 Ba3 Ir1 93.3(2) 7_546 1_556
O4 Ba3 Ir1 93.3(2) 7_556 1_556
O5b Ba3 Ir1 114.020(19) 1_556 1_556
O5b Ba3 Ir1 114.020(19) 6_556 1_556
Al1 Ba3 Ir1 134.61(8) 1_556 1_556
O5a Ba4 O5a 52.814(15) . 6
O5a Ba4 O2 150.38(7) . 5_556
O5a Ba4 O2 150.38(7) 6 5_556
O5a Ba4 O3 140.67(11) . 6
O5a Ba4 O3 110.02(10) 6 6
O2 Ba4 O3 62.82(16) 5_556 6
O5a Ba4 O3 110.02(10) . .
O5a Ba4 O3 140.67(11) 6 .
O2 Ba4 O3 62.82(16) 5_556 .
O3 Ba4 O3 58.0(2) 6 .
O5a Ba4 O5b 17.176(4) . 7_556
O5a Ba4 O5b 64.552(17) 6 7_556
O2 Ba4 O5b 143.689(14) 5_556 7_556
O3 Ba4 O5b 128.83(11) 6 7_556
O3 Ba4 O5b 93.10(10) . 7_556
O5a Ba4 O5b 64.552(17) . 4_546
O5a Ba4 O5b 17.176(4) 6 4_546
O2 Ba4 O5b 143.689(13) 5_556 4_546
O3 Ba4 O5b 93.10(10) 6 4_546
O3 Ba4 O5b 128.83(11) . 4_546
O5b Ba4 O5b 72.459(19) 7_556 4_546
O5a Ba4 O1 59.5(2) . 7_556
O5a Ba4 O1 111.4(2) 6 7_556
O2 Ba4 O1 92.1(2) 5_556 7_556
O3 Ba4 O1 129.1(2) 6 7_556
O3 Ba4 O1 71.3(2) . 7_556
O5b Ba4 O1 52.9(2) 7_556 7_556
O5b Ba4 O1 123.9(2) 4_546 7_556
O5a Ba4 O1 111.4(2) . 7_546
O5a Ba4 O1 59.5(2) 6 7_546
O2 Ba4 O1 92.1(2) 5_556 7_546
O3 Ba4 O1 71.3(2) 6 7_546
O3 Ba4 O1 129.1(2) . 7_546
O5b Ba4 O1 123.9(2) 7_556 7_546
O5b Ba4 O1 52.9(2) 4_546 7_546
O1 Ba4 O1 158.2(4) 7_556 7_546
O5a Ba4 O2 79.70(12) . .
O5a Ba4 O2 79.70(12) 6 .
O2 Ba4 O2 87.6(2) 5_556 .
O3 Ba4 O2 136.55(14) 6 .
O3 Ba4 O2 136.55(14) . .
O5b Ba4 O2 94.06(11) 7_556 .
O5b Ba4 O2 94.06(11) 4_546 .
O1 Ba4 O2 79.4(2) 7_556 .
O1 Ba4 O2 79.4(2) 7_546 .
O5a Ba4 Ir1 145.54(2) . .
O5a Ba4 Ir1 145.54(2) 6 .
O2 Ba4 Ir1 36.91(16) 5_556 .
O3 Ba4 Ir1 35.59(10) 6 .
O3 Ba4 Ir1 35.59(10) . .
O5b Ba4 Ir1 128.47(2) 7_556 .
O5b Ba4 Ir1 128.47(2) 4_546 .
O1 Ba4 Ir1 98.06(19) 7_556 .
O1 Ba4 Ir1 98.06(19) 7_546 .
O2 Ba4 Ir1 124.50(14) . .
O5a Ba4 Al1 31.03(6) . 7_556
O5a Ba4 Al1 83.52(6) 6 7_556
O2 Ba4 Al1 120.35(8) 5_556 7_556
O3 Ba4 Al1 142.59(12) 6 7_556
O3 Ba4 Al1 89.04(12) . 7_556
O5b Ba4 Al1 26.65(7) 7_556 7_556
O5b Ba4 Al1 95.46(7) 4_546 7_556
O1 Ba4 Al1 28.5(2) 7_556 7_556
O1 Ba4 Al1 139.8(2) 7_546 7_556
O2 Ba4 Al1 79.02(10) . 7_556
Ir1 Ba4 Al1 122.08(6) . 7_556
O5b Al1 O5b 105.7(3) 6 .
O5b Al1 O1 103.7(3) 6 .
O5b Al1 O1 103.7(3) . .
O5b Al1 O4 113.0(3) 6 .
O5b Al1 O4 113.0(3) . .
O1 Al1 O4 116.6(6) . .
O5b Al1 O5a 26.556(15) 6 4_546
O5b Al1 O5a 130.7(3) . 4_546
O1 Al1 O5a 101.66(14) . 4_546
O4 Al1 O5a 91.57(15) . 4_546
O5b Al1 O5a 130.7(3) 6 7_556
O5b Al1 O5a 26.556(15) . 7_556
O1 Al1 O5a 101.66(14) . 7_556
O4 Al1 O5a 91.57(15) . 7_556
O5a Al1 O5a 152.1(3) 4_546 7_556
O5b Al1 Ba3 74.87(16) 6 1_554
O5b Al1 Ba3 74.87(16) . 1_554
O1 Al1 Ba3 177.4(5) . 1_554
O4 Al1 Ba3 65.9(4) . 1_554
O5a Al1 Ba3 78.01(14) 4_546 1_554
O5a Al1 Ba3 78.01(14) 7_556 1_554
O5b Al1 Ba2 65.27(13) 6 .
O5b Al1 Ba2 65.27(13) . .
O1 Al1 Ba2 66.9(4) . .
O4 Al1 Ba2 176.5(5) . .
O5a Al1 Ba2 87.59(12) 4_546 .
O5a Al1 Ba2 87.59(12) 7_556 .
Ba3 Al1 Ba2 110.58(14) 1_554 .
O5b Al1 Ba1 126.64(13) 6 .
O5b Al1 Ba1 126.64(13) . .
O1 Al1 Ba1 58.1(4) . .
O4 Al1 Ba1 58.6(4) . .
O5a Al1 Ba1 102.64(13) 4_546 .
O5a Al1 Ba1 102.64(13) 7_556 .
Ba3 Al1 Ba1 124.48(13) 1_554 .
Ba2 Al1 Ba1 124.95(14) . .
O5b Al1 Ba4 134.90(19) 6 7_556
O5b Al1 Ba4 51.13(9) . 7_556
O1 Al1 Ba4 58.27(10) . 7_556
O4 Al1 Ba4 111.90(19) . 7_556
O5a Al1 Ba4 153.88(18) 4_546 7_556
O5a Al1 Ba4 43.46(7) 7_556 7_556
Ba3 Al1 Ba4 121.24(7) 1_554 7_556
Ba2 Al1 Ba4 69.66(7) . 7_556
Ba1 Al1 Ba4 81.49(9) . 7_556
O5b Al1 Ba4 51.13(9) 6 7_546
O5b Al1 Ba4 134.90(19) . 7_546
O1 Al1 Ba4 58.27(10) . 7_546
O4 Al1 Ba4 111.90(19) . 7_546
O5a Al1 Ba4 43.46(7) 4_546 7_546
O5a Al1 Ba4 153.88(18) 7_556 7_546
Ba3 Al1 Ba4 121.24(7) 1_554 7_546
Ba2 Al1 Ba4 69.66(7) . 7_546
Ba1 Al1 Ba4 81.49(9) . 7_546
Ba4 Al1 Ba4 113.56(12) 7_556 7_546
O5b Al1 Ba3 65.67(7) 6 7_546
O5b Al1 Ba3 151.0(2) . 7_546
O1 Al1 Ba3 105.3(3) . 7_546
O4 Al1 Ba3 53.81(5) . 7_546
O5a Al1 Ba3 39.93(7) 4_546 7_546
O5a Al1 Ba3 143.09(17) 7_556 7_546
Ba3 Al1 Ba3 76.10(7) 1_554 7_546
Ba2 Al1 Ba3 126.12(5) . 7_546
Ba1 Al1 Ba3 72.02(7) . 7_546
Ba4 Al1 Ba3 153.51(14) 7_556 7_546
Ba4 Al1 Ba3 62.92(3) 7_546 7_546
Al1 O1 Ba1 90.2(4) . .
Al1 O1 Ba1 169.7(7) . 5_656
Ba1 O1 Ba1 100.1(4) . 5_656
Al1 O1 Ba2 81.5(5) . .
Ba1 O1 Ba2 171.6(5) . .
Ba1 O1 Ba2 88.3(3) 5_656 .
Al1 O1 Ba4 93.3(3) . 7_556
Ba1 O1 Ba4 100.4(2) . 7_556
Ba1 O1 Ba4 85.0(2) 5_656 7_556
Ba2 O1 Ba4 80.2(2) . 7_556
Al1 O1 Ba4 93.3(3) . 7_546
Ba1 O1 Ba4 100.4(2) . 7_546
Ba1 O1 Ba4 85.0(2) 5_656 7_546
Ba2 O1 Ba4 80.2(2) . 7_546
Ba4 O1 Ba4 158.2(4) 7_556 7_546
Ir1 O2 Ba4 92.6(3) 1_556 5_556
Ir1 O2 Ba3 92.8(3) 1_556 .
Ba4 O2 Ba3 174.6(3) 5_556 .
Ir1 O2 Ba1 85.61(14) 1_556 7_546
Ba4 O2 Ba1 88.47(14) 5_556 7_546
Ba3 O2 Ba1 91.94(14) . 7_546
Ir1 O2 Ba1 85.61(14) 1_556 7_556
Ba4 O2 Ba1 88.47(14) 5_556 7_556
Ba3 O2 Ba1 91.94(14) . 7_556
Ba1 O2 Ba1 170.6(3) 7_546 7_556
Ir1 O2 Ba4 175.0(3) 1_556 .
Ba4 O2 Ba4 92.4(2) 5_556 .
Ba3 O2 Ba4 82.22(19) . .
Ba1 O2 Ba4 94.53(14) 7_546 .
Ba1 O2 Ba4 94.53(14) 7_556 .
Ir1 O3 Ba2 172.6(3) . 7_556
Ir1 O3 Ba1 93.23(18) . 3_455
Ba2 O3 Ba1 93.82(15) 7_556 3_455
Ir1 O3 Ba4 88.59(18) . .
Ba2 O3 Ba4 89.32(15) 7_556 .
Ba1 O3 Ba4 89.50(15) 3_455 .
Ir1 O3 Ba3 89.36(18) . 1_554
Ba2 O3 Ba3 84.02(13) 7_556 1_554
Ba1 O3 Ba3 170.6(2) 3_455 1_554
Ba4 O3 Ba3 99.56(16) . 1_554
Ir1 O3 Ba1 90.23(18) . 7
Ba2 O3 Ba1 93.13(15) 7_556 7
Ba1 O3 Ba1 79.81(13) 3_455 7
Ba4 O3 Ba1 169.2(2) . 7
Ba3 O3 Ba1 91.19(15) 1_554 7
Al1 O4 Ba2 174.8(6) . 1_554
Al1 O4 Ba1 89.5(5) . .
Ba2 O4 Ba1 95.7(4) 1_554 .
Al1 O4 Ba3 81.7(5) . 1_554
Ba2 O4 Ba3 93.0(3) 1_554 1_554
Ba1 O4 Ba3 171.2(5) . 1_554
Al1 O4 Ba3 99.0(2) . 7_546
Ba2 O4 Ba3 81.0(2) 1_554 7_546
Ba1 O4 Ba3 90.0(2) . 7_546
Ba3 O4 Ba3 91.4(2) 1_554 7_546
Al1 O4 Ba3 99.0(2) . 7_556
Ba2 O4 Ba3 81.0(2) 1_554 7_556
Ba1 O4 Ba3 90.0(2) . 7_556
Ba3 O4 Ba3 91.4(2) 1_554 7_556
Ba3 O4 Ba3 162.0(5) 7_546 7_556
O5b O5a Al1 58.79(13) 7_556 7_556
Al1 O5a Ba4 105.51(13) 7_556 .
O5b O5a Ba3 161.647(12) 7_556 .
Al1 O5a Ba3 111.34(12) 7_556 .
Ba4 O5a Ba3 96.23(2) . .
Al1 O5a Ba2 129.09(14) 7_556 .
Ba4 O5a Ba2 104.83(2) . .
Ba3 O5a Ba2 104.812(16) . .
O5a O5b Al1 94.66(12) 7_556 .
Al1 O5b Ba2 156.08(15) . 7_556
Al1 O5b Ba4 102.22(15) . 7_556
Ba2 O5b Ba4 98.664(16) 7_556 7_556
Al1 O5b Ba2 84.20(13) . .
Ba2 O5b Ba2 109.469(12) 7_556 .
Ba4 O5b Ba2 84.506(17) 7_556 .
Al1 O5b Ba3 75.11(15) . 1_554
Ba2 O5b Ba3 81.053(15) 7_556 1_554
Ba4 O5b Ba3 155.780(19) 7_556 1_554
Ba2 O5b Ba3 118.631(13) . 1_554
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ir1 O3 1.970(5) 5
Ir1 O3 1.970(5) .
Ir1 O3 1.970(5) 2
Ir1 O3 1.970(5) 6
Ir1 O2 2.034(7) 5_556
Ir1 O2 2.034(7) 1_554
Ir1 Ba4 3.3833(7) 5
Ir1 Ba4 3.3833(7) .
Ir1 Ba3 3.4497(6) 5_556
Ir1 Ba3 3.4497(6) 1_554
Ir1 Ba1 3.4848(4) 3_455
Ir1 Ba1 3.4848(4) 7_545
Ba1 O1 2.743(12) .
Ba1 O4 2.757(11) .
Ba1 O1 2.761(11) 5_656
Ba1 O3 2.766(5) 8
Ba1 O3 2.766(5) 3_545
Ba1 O3 2.867(5) 4_545
Ba1 O3 2.867(5) 7
Ba1 O2 2.9897(6) 7_546
Ba1 O2 2.9897(6) 7_556
Ba1 Al1 3.232(5) .
Ba1 Ir1 3.4848(4) 3_545
Ba1 Ir1 3.4848(4) 3
Ba2 O5b 2.5357(4) 4_546
Ba2 O5b 2.5357(4) 7_556
Ba2 O5a 2.6059(5) 6
Ba2 O5a 2.6059(5) .
Ba2 O4 2.708(12) 1_556
Ba2 O3 2.712(5) 7_556
Ba2 O3 2.712(5) 4_546
Ba2 O5b 2.9239(6) 6
Ba2 O5b 2.9239(6) .
Ba2 O1 2.978(13) .
Ba2 Al1 3.203(4) .
Ba2 Ba3 3.7268(6) 7_557
Ba3 O5a 2.5442(6) 6
Ba3 O5a 2.5442(6) .
Ba3 O2 2.688(7) .
Ba3 O3 2.854(5) 6_556
Ba3 O3 2.854(5) 1_556
Ba3 O4 2.913(12) 1_556
Ba3 O4 3.017(2) 7_546
Ba3 O4 3.017(2) 7_556
Ba3 O5b 3.1538(7) 1_556
Ba3 O5b 3.1538(7) 6_556
Ba3 Al1 3.157(5) 1_556
Ba3 Ir1 3.4497(6) 1_556
Ba4 O5a 2.5425(6) .
Ba4 O5a 2.5425(6) 6
Ba4 O2 2.615(7) 5_556
Ba4 O3 2.800(5) 6
Ba4 O3 2.800(5) .
Ba4 O5b 2.8371(6) 7_556
Ba4 O5b 2.8371(6) 4_546
Ba4 O1 3.034(2) 7_556
Ba4 O1 3.034(2) 7_546
Ba4 O2 3.057(7) .
Ba4 Al1 3.562(2) 7_556
Al1 O5b 1.635(3) 6
Al1 O5b 1.635(3) .
Al1 O1 1.701(13) .
Al1 O4 1.708(13) .
Al1 O5a 1.9051(12) 4_546
Al1 O5a 1.9051(12) 7_556
Al1 Ba3 3.157(5) 1_554
Al1 Ba4 3.562(2) 7_556
Al1 Ba4 3.562(2) 7_546
Al1 Ba3 3.692(2) 7_546
O1 Ba1 2.761(11) 5_656
O1 Ba4 3.034(2) 7_556
O1 Ba4 3.034(2) 7_546
O2 Ir1 2.034(7) 1_556
O2 Ba4 2.615(7) 5_556
O2 Ba1 2.9897(6) 7_546
O2 Ba1 2.9897(6) 7_556
O3 Ba2 2.712(5) 7_556
O3 Ba1 2.766(5) 3_455
O3 Ba3 2.854(5) 1_554
O3 Ba1 2.867(5) 7
O4 Ba2 2.708(12) 1_554
O4 Ba3 2.913(12) 1_554
O4 Ba3 3.017(2) 7_546
O4 Ba3 3.017(2) 7_556
O5a O5b 0.8545 7_556
O5a Al1 1.9051(12) 7_556
O5b O5a 0.8545 7_556
O5b Ba2 2.5357(4) 7_556
O5b Ba4 2.8371(6) 7_556
O5b Ba3 3.1538(7) 1_554
